welding temperature. Further, it should have a good oxidation resistance and a low thermal conductivity to minimise heat loss and thermal damage to the machinery further up the drive train. Hot-worked tool steel such as AISI H13 has proven perfectly acceptable for welding aluminium alloys within thickness ranges of 0.5–50 mm but more advanced tool materials are necessary for more demanding applications such as highly abrasive metal matrix composites or higher-melting-point materials such as steel or titanium. Improvements in tool design have been shown to cause substantial improvements in productivity and quality. TWI has developed tools specifically designed to increase the penetration depth and thus increasing the plate thicknesses that can be successfully welded. An example is the "whorl" design that uses a tapered pin with re-entrant features or a variable-pitch thread to improve the downwards flow of material. Additional designs include the Triflute and Trivex series. The Triflute design has a complex system of three tapering, threaded re-entrant flutes that appear to increase material movement around the tool. The Trivex tools use a simpler, non-cylindrical, pin and have been found to reduce the forces acting on the tool during welding. The majority of tools have a concave shoulder profile, which acts as an escape volume for the material displaced by the pin, prevents material from extruding out of the sides of the shoulder and maintains downwards pressure and hence good forging of the material behind the tool. The Triflute tool uses an alternative system with a series of concentric grooves machined into the surface, which are intended to produce additional movement of material in the upper layers of the weld. Widespread commercial applications of friction stir welding process for steels and other hard alloys such as titanium alloys will require the development of cost-effective and durable tools. Material selection, design and cost are important considerations in the search for commercially useful tools for the welding of hard materials. Work is continuing to better understand the effects of tool material's composition, structure, properties and geometry on their performance, durability and cost. Tool rotation and traverse speeds There are two tool speeds to be considered in friction-stir welding; how fast the tool rotates and how quickly it traverses along the interface. These two parameters have considerable importance and must be chosen with care to ensure a successful and efficient welding cycle. The relationship between the rotation speed, the welding speed and